PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES


 Octavia Shelton
 1 years ago
 Views:
Transcription
1 THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile Engineering, Department of Textile Evaluation, Czech Republic Keywords: Layered structures, elastic properties, finite element analysis (FEA), prepreg 1 Introduction The article deals with multiscale modelling in threedimensional model. Main focus was concerned to the mesolevel which is in our case the basic unit cell of plain weave reinforcement consists from cross linked infinite fibre bundles. Construction of models allows classical weave of woven reinforcement but also slides places during lamination process and curing. Anyway some idealization was also necessary in study of its symmetry. Composites with textile reinforcement have got good resistance against to progression of cracks and give good tensile properties in warp and weft directions. However the structure modelling of composites is than a complex problem. Here is irregularly crimped textile reinforcement with various inherent defects (pores, bubbles and cracks) which has risen during pyrolysis process of polymer precursor in carbon matrix. Different shrinkage during cooling plays its role too [1, 2]. Lamination gives to the structure imperfection in faze of woven reinforcement thus defects can rise in areas full of matrix whereas same direction bundles lie on each other. It is difficult to include all aspects of this complex structure to one model. The idealisation is based on geometric models as the bricks or sinusoidal curve of woven reinforcement [3, 4]. Composites with weave reinforcement structure were studied by image analysis at the Technical University of Liberec. 1.1 Material Material was set on carbon/carbon composite which was already tested with classical tests so results should be proved and corrected. Fig. 1. Image of woven reinforcement composite crosssection example 1 view of interlace Fig. 2. Image of woven reinforcement composite crosssection example 2 view of vacuole Presented results are based on carbon material input values. The real composite, our tested material for real image structure observation, was made from carbon materials. Carbon and carbon fibres have got unique properties. Carbon fibres embody special alternatives in
2 symmetry. If we compare carbon in various stages with other materials we can find high correlation of Young s modulus on density. Different materials were metal, wood, elements, glass, rubber, porcelain etc. Density and Young s modulus correlation for various basic materials is minimal. However line for glassy carbon, graphite and diamond correlate very high, see Fig. 3. Mass density and Young s modulus for materials were gathered mainly from internet research on Web of Knowledge, Google, Science Direct from journal articles and product material sheets. Fig. 3. Correlation densityyoung s modulus for different common materials and carbons When we compare basic carbons with carbon fibres correlation we find even higher dependency between mass density and Young s modulus. Fig. 4. gives us this relation clear. Fibres not only from carbon are highly oriented along the structure because of the process spinning from spinneret. Fibre is extruded through the thin spinneret and orientation along the fibre axis organizes bonds inside the fibre in this preferable direction. We use it as a benefit for composite construction. Bundles multiply reinforcing effect and weaving spread this effect to the symmetry in two directions across. Fig. 4. Correlation densityyoung s modulus for carbons and carbon fibres We based our modelling on the real composite prepared by prepreg technology. The tested composite was layered laminate from carbon fibre in plain weave surrounded with carbon matrix. Fibres were graphitized so the structure is highly oriented along fibre axis with transversal isotropy symmetry presumption. Matrix was prepared from phenolic resin with hightemperature treatment to the carbonized temperature so the presumption is that matrix has got glassy carbon structure with isotropic orientation. Bundle is made from 6000 parallel infinite high strength carbon fibres. Important input properties are in Table 1. Component Density [kg.m 3 ] Young s modulus [MPa] Poisson s ratio [] Fibres ,24 Matrix ,30 Voids  air 1,3 0,0 0,0 Table 1 Values of important input mechanical properties The computation without a plastic deformation by scanning of stress and strain concentrations and it is also possible to evaluate elastic constants. An alternative model for determining properties of future composite construction is a calculation which we do with commercial software. The structure modelling in multiscale supports calculation in finite element method effectively.
3 PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES 2 Models and Computation 2.1 Multiscale modelling The multiscale modelling allows decomposition of complex heterogeneous structure to the partial levels from the simplest composition to the composition of whole sample body. The main sources for the theory equations and relations were work of Berthelot [5], Bogdanovich [4], Lomov [3] and Miravete [6]. Bogdanovich 3D mosaic model should describe basic idea of composition when computation from lower level are used in higher level as an local input of the complex higher structure [4]. Original research of Bogdanovich ([4] Bognanovich A.E.: Threedimensioanl variation theory of laminated composite plates and its implementation with Bernstein basis function. Comput. Methods Appl. Engrg , Elsevier, 2000.) was used as a key theory source also in the previous research of author of this paper in 2D modelling presented by TěšinováVozková, Salačová in "Elastic Properties of Woven Composite" published at the Comsol Users Conference 2006 Prague. In this earlier work the model described on page 1 belongs to the Prof. Bogdanovich and the reference was missed in the text by mistake. 2.2 Model Description On Fig. 6. is parting to the scales. A simulation in our case presents the twodimensional model and threedimensional model of lengthwise and crosswise fibre bundles surrounded with matrix. Defects are mentioned here, too. It is necessary to include defects in the bundles, between laminas and voids raised during pyrolysis and layering. Whole structure is a combination of geometry formations. Modelling is described in more detail in literature [7, 8]. Fig. 6. Multiscale models in 2D: fibre + matrix, bundle + defects, periodic unit cells, lamina [7] Fig. 5. Brick nomenclature in 3D mosaic model by Bogdanovich [4] Fig. 7. Multiscale models in 3D: fibre + matrix, bundle + defects, periodic unit cells, lamina [8] 3
4 Composite is composed from bundles crosslinked in the woven structure and based lamina. Whole composite is that constructed simply by two types of lamina to the plain structure. We study preferably composites in plain because of the simplicity of formulation of results and because we are focused to the structure. Pure mechanical description can count with selection of "black box" and have good results for composite, but it is mainly based on experiment. We work with real composites to obtain inside structure of the reinforcement and try to idealize as less as possible. Scale and type of the tested sample length [m] high [m] Crosswise bundle 2, , Lengthwise bundle 2, , Crosswise bundle with defects 1, , Lengthwise bundle section with defects 1, , Structure unit cell 1 4, , Structure unit cell 2 4, , Lamina 1 0,0315 0, Lamina 2 0,0315 0, ,0315 1, Table 2 Multiscale model dimensions In our multiscale model it is counted with whole model in stages from fibres to bundles but in previous research we used third type of basic unit cell which we now neglected because our recommended composites contain (with pressure 0.5 MPa for 6 layers) just two basic types of basic unit cell: without defects in proper layout and in translation where defects are inside the structure. Optimal number of defects is occurred in type of composites. 2.3 Software Used For Computation In the experiment here is a description of the results obtained from the simulation in Comsol MultiphysicsTM. which is used for calculation with proper determination of the material properties, boundary states and net adjusting. 2.4 Model Presumptions Sample was clamped on one side and loaded in the axis x thus model was tested for simple stress strain characteristic in elastic area of loading to find elastic modulus. 2.5 Stress Concentrations in Models The longitudinal stress of fibrematrix focus to bundle is concentrated in the fibres and stressed mostly where fibres are close to each other and matrix cannot spread loading so effectively. Mean stress is in the middle of the fibres. The crosswise bundle with defects has got the highest longitudinal stress in the carbon part near defects horizontal curvature. A minimum is everywhere else. The concentration of the stress and of the strain is highly affected by the occurrence of the defects in the carbon part. The carbon part carries stress and the pores localize strain. Unit cell level is described with the following figures. Structure unit cell 1 concentrates stress in whole bundle. This bundle is lengthwise to the loading. Maximum stress is located in the parts which hold the loading longitudinal. However stress is not the same in all area of the bundle. It is caused by the higher stress in the thinner sample place of further area. It caused that stress from tension is than not located in the centre of the bundle length but close the contact point. When we focus to the axis x we can observe maximal loading in the curvature and changing of the curvature where bundle goes from one binding point to the next and is than surrounded only with the matrix. Holding of the load is mostly on the fibres here and matrix only spread tension to the neighbouring fibres and bundles. For better predicative of relation matrix was not visualised but loading was not on maximum at that parts. Fig. 8. stress computation in visualisation of crosssection in axis z
5 PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES Fig. 9. stress computation in visualisation of crosssection in axis x Anyway maximal loaded area was observed in the middle of the structure in the bundle where curvature if the bundle changed from one contact point to the next. Next the higher stress is located in the curvature places where contact surfaces with bundles with cross direction on that position. Defects embodies tendency to the deformation and strain is located in them. Matrix surrounded defects is than under the tension and spread loading to the neighbouring part of the bundle so it is the more reason why lengthwise bundles are at maximum loading when they are surrounded by matrix in this scale of model. The unit cell 1 has got more balanced loading for the stress properties than unit cell 2. The longitudinal stress is high here but not really critical for both, we are still in the elastic relations without deformation so we detected only tension no plastic deformation. Curvature and matrix apply a load to the lengthwise bundles the most. Also cross bundles affects not allowance against flotation. Fig. 12. stress computation in visualisation of crosssection in axis z Laminas have got the highest stress and strain in the whole area. The lamina is combined from bricks with the same parameters so these results are expected. The whole composite combined from laminas has got longitudinal stress close to the clamped end of the sample similarly like single lamina. The higher impact goes farther for lamina which it has got higher longitudinal stress from the previous single testing. But impact is the same no matter which lamina it is. 3 Results and discussion Simulations with the finite element method are fast and precise same as a resonant oscillation experiment. Both methods were compared. Relations in following graphs were interpolated with equation included calculation of axis in plane [9]. Loading in on axis direction has to be transferred to the symmetry axis in defined angle δ []. Loading is then transferred to the main directions. Longitudinal modulus could be defined with inclusion constants from compliance tensor [9] LT 2 2 cos sin ( )cos sin E E E G E x L T LT L (1) where E x is longitudinal modulus in any angle [Pa], E L is Young s modulus [Pa], E T is transversal modulus [Pa], G LT is shear modulus [Pa], µ LT is Poisson s ratio [], angle δ is varied in whole 360 in plane of reinforcement through warp and weft twice [9]. Fig. 10. stress computation in visualisation of crosssection in axis x 5
6 E G G ' G xy 2 sin cos sin cos 1 (2) where E, G and μ are Young s modulus, shear modulus and Poisson number for xy axis inplane where axis X 1 has go direction of warp [9]. Experiment was tested at Department of Structure and Mechanics of Rocks of Science Academy of the Czech Republic and was used as a special comparing property for the multiscale simulation [9]. Fig. 13. Young s modulus for carbonised composite samples from eigen frquency experiment Fig. 14. Young s modulus for graphitised composite samples from eigen frquency experiment The experiment was compared with a simulation and it is visualized in diagrams for the inplane treatment in the plain weave reinforcement. Model was set as clamped on left side in the axis x and loaded for tensile test along axis x. Only axis x was in deformation to elongation, the other sides should be on shrinkage because no other restrictions for roll of fix on the sided of model to test as close to real experiment as possible. Scale and type of the tested sample 2D 3D Composite from experiment from simulation 2D from simulation 3D Longitudinal modulus for warp[mpa] Model axis x <56332;53294> <64104;60646> <39842;37693> <51130;48372> <105854;100145> <88350;83585> <105118;99447> Table 3 Values of mechanical properties Longitudinal modulus for warp [MPa] Scale and type of the tested sample 2D 3D Transversal modulus [MPa] Model axis y 408 <419;397> 717 <736;697> 3056 <3140;2971> 3782 <3886;3677> Composite from experiment from simulation 2D <587;556> 3444 from simulation 3D <3539;3348> Table 4 Values of mechanical properties Transversal modulus inplane of textile [MPa]
7 PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES Scale and type of the tested sample 2D 3D Composite from experiment from simulation 2D from simulation 3D Longitudinal modulus for weft [MPa] Model axis z <56332;53293> <64103;60646> <45052;42621> <49141;46490> <110993;105006> <88350;83585> <108929;103054> Table 5 Values of mechanical properties  Longitudinal modulus for weft [MPa] probable. Though this, let say, disadvantage is getting better results in the higher levels. In lamina and in the composite body is 3D the reason why whole composite longitudinal modulus is a bit better to 2D type of model. In this type of model where we count it as a one component loading is better to be transferred to the directions and results are getting higher. Anyway this difference is not critical and both results are comparable and with good agreement with the experiment. Fig. 15. Unit cell longitudinal modulus computed from various methods and models in comparison Unit cell level in 2D model occurs a bit higher values of the longitudinal modulus but it is caused mainly by the model. Loading should be spread only to the two dimensions thus one lengthwise bundle or two in the only one direction hold the loading as predicted. In the 3D model loading is spread to the sample and curvature or more matrix amount in the sample body. The presence of the weak point is more Fig. 16. Whole composite longitudinal modulus computed from various methods, models and experiment in comparison The conclusion from the previous pages follows as estimation between the experiment and the simulation of elastic properties of the carbon/carbon composite with the plain weave reinforcement. We used models in two types 2D and 3D. The simulation and experiment correlate well for longitudinal modulus of the whole composite in all directions in the inplane of the reinforcement, for 3D model even better than 2D. The theory agrees well for it where warp and weft reinforce composite greatly. The simulation was adapted quite well for the real composite. Combination of the multiscale and the finite element simulation provide relevant data of the elastic modules which is confirmed by the used experiment. More directions are offered to the evaluation and not only isotropic structure is possible to be used. 7
8 3 Conclusion Simulation helps to evaluate properties in longitudinal and also in the transversal directions for material with an orthotropic properties. The simulation with the multiscale modelling is necessary to evaluate precise input values for the lowest scale. Simulation helps to evaluate properties in longitudinal and also in the transversal directions for material with an orthotropic properties. More directions are offered to the evaluation and not only isotropic structure is possible to be used. It is an advantage of the experiment. Some more advanced sample preparing should be done in the future for making thin plates in different directions of the composite especially for the direction transversely to the reinforcement. The most influencing factor for the elastic properties is an amount of the lengthwise bundles, the position of the crosswise bundles with the matrix properties and of the defects. Defects work upon all others modulus too. The simulation with the multiscale modelling is necessary to evaluate precise input values for the lowest scale. Here it is not problem with the fibre testing. Many methods are used and suitable. The matrix properties are more complicated to obtain and it is necessary to be patient and precise in determination. Previous nondestructive testing is possible to use for any material with the similar structure and the same prepreg technology. If geometry models on the Periodic unit cell scale are adapted, different technology should be evaluated with the same procedure too. Both methods presented here, the experiment and the finite element simulation, are good instrument together for the testing of the elastic properties and preparing of the new composites with varied structure or material properties. It is also useful to compute from whole structure with defined end properties and find out components with ability to construct. Acknowledgements The work was financially supported by the grant GA106/09/P648 of the Czech Science Foundation. References [1] Savage, G. (1993). CarbonCarbon Composites. Chapman and Hall, ISBN , London, UK [2] Fitzer, E.; Manocha, L.M. (1998). Carbon reinforcement and CarbonCarbon Composites. Springer Verlag, ISBN Berlin, Germany [3] Lomov, S. V., G. Perie, D. S. Ivanov, I. Verpoest and D. Marsal (2011). "Modelling 3D fabrics and 3D reinforced composites: Challenges and solutions." Textile Research Journal, 81(1), p [4] Bognanovich A.E.: Threedimensioanl variation theory of laminated composite plates and its implementation with Bernstein basis function. Comput. Methods Appl. Engrg , Elsevier, [5] Berthelot, J.M. (1999). Composite Materials. Mechanical Behavior and Structural Analysis. SpringerVerlag, ISBN , New York, USA [6] Miravete, A. 3D textile reinforcements in composite materials. Book of contributors. Woodhead Publishing Ltd Cambridge England and CRC Press, ISBN , Cambridge, UK, (2000). [7] Vozková, P.: Elastic modulus FEM modelling of the layered woven composite material. kapitola v knize Recent Advances in Modelling and Simulation. Editor: Petrone and Cammarata. ITech Education and Publishing, Vienna, Austria, ISBN [8] TESINOVA, P.. Mechanical properties computed from 3D models of textile composites based on real structures. Bulletin of Applied Mechanics, North America, 7, dec Available at: Date accessed: 10 Jan ISSN [9] Černý, M.; Glogar, P.; Manocha, L.M.: Resonant frequency study of tensile and shear moduli of carbon fibre reinforced composites. Pergamon, Carbon 38 (2000)
ScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationFeatures and design of elastomer / textile engineered structures. D Boast, C Eng. F Mech E.
Features and design of elastomer / textile engineered structures D Boast, C Eng. F Mech E. Title of meeting IOM Bla blah Topics Materials: Environmental acids, water, oil, radiation etc. Bonding. Cost.
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationOptical Measurement of the Springback Angle of Composite Plates
Optical Measurement of the Springback Angle of Composite Plates Zdeněk Padovec 1, Milan Růžička 2, Milan Dvořák 3, Vladimír Stavrovský 4 & Hynek Chlup 5 Abstract: Presented paper describes measurement
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationFEM Modeling of a 3D Printed Carbon Fiber Pylon
FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationFINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE
FINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE NEHME Samer *, HAGEGE Benjamin *, KAABI Abderrahmen **, BENZEGGAGH Malk * * Université de Technologie de Compiègne,
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationTwodimensional ternary locally resonant phononic crystals with a comblike coating
Twodimensional ternary locally resonant phononic crystals with a comblike coating YanFeng Wang, YueSheng Wang,*, and Litian Wang Institute of Engineering Mechanics, Beijing Jiaotong University, Beijing,
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationChapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING )
Chapter 5 CENTRIC TENSION OR COMPRESSION ( AXIAL LOADING ) 5.1 DEFINITION A construction member is subjected to centric (axial) tension or compression if in any cross section the single distinct stress
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationConcrete Technology Prof. B. Bhattacharjee Department of Civil Engineering Indian Institute of Technology, Delhi
Concrete Technology Prof. B. Bhattacharjee Department of Civil Engineering Indian Institute of Technology, Delhi Lecture  25 Strength of Concrete: Factors Affecting Test Results Welcome to module 6, lecture
More informationModelling of viscoelastic properties of a curing adhesive
Computational Methods and Experiments in Materials Characterisation III 241 Modelling of viscoelastic properties of a curing adhesive J. de Vreugd 1, K. M. B. Jansen 1, L. J. Ernst 1 & J. A. C. M. Pijnenburg
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationSTRUCTURAL OPTIMIZATION OF A MATERIAL EXHIBITING NEGATIVE STIFFNESS
International Conference on Engineering Vibration Ljubljana, Slovenia, 70 September 05 STRUCTURAL OPTIMIZATION OF A MATERIAL EXHIBITING NEGATIVE STIFFNESS Zuzana Dimitrovová*, Jan Heczo, Helder C. Rodrigues
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationBolted Busbar Connections with Slotted Bolt Holes
Bolted Busbar Connections with Slotted Bolt Holes RAINA TZENEVA 1, YANKO SLAVTCHEV 2 and VALERI MLADENOV 3 1 Department of Electrical Apparatus, Faculty of Electrical Engineering, Technical University
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationEXPERIMENTAL ANALYSIS OF THE TENSILE PROPERTIES OF PAINTING CANVAS
AUTEX Research Journal, DOI: 1.1515/aut21523 AUTEX EXPERIMENTAL ANALYSIS OF THE TENSILE PROPERTIES OF PAINTING CANVAS Željko Penava 1 *, Diana Šimić Penava 2, Marijana Tkalec 1 1 University of Zagreb,
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationMultiscale modeling of failure in ABS materials
Institute of Mechanics Multiscale modeling of failure in ABS materials Martin Helbig, Thomas Seelig 15. International Conference on Deformation, Yield and Fracture of Polymers Kerkrade, April 2012 Institute
More informationσ = F/A ε = L/L σ ε a σ = Eε
Material and Property Information This chapter includes material from the book Practical Finite Element Analysis. It also has been reviewed and has additional material added by Sascha Beuermann. Hooke
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationA MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE
A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE 2014 A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationThe Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar
The Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar DUMITRU BOLCU 1 *, MIHAELA SAVA 2, ALIN DINITA 3, COSMIN
More informationSENSITIVITY ANALYSIS OF LATERAL BUCKLING STABILITY PROBLEMS OF HOTROLLED STEEL BEAMS
2005/2 PAGES 9 14 RECEIVED 18.10.2004 ACCEPTED 18.4.2005 Z. KALA, J. KALA SENSITIVITY ANALYSIS OF LATERAL BUCKLING STABILITY PROBLEMS OF HOTROLLED STEEL BEAMS ABSTRACT Doc. Ing. Zdeněk KALA, PhD. Brno
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationElasticity: Term Paper. Danielle Harper. University of Central Florida
Elasticity: Term Paper Danielle Harper University of Central Florida I. Abstract This research was conducted in order to experimentally test certain components of the theory of elasticity. The theory was
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 3 VISCOELASTICITY. k a. N t
MATERIAL MECHANICS, SE2126 COMPUTER LAB 3 VISCOELASTICITY N t i Gt () G0 1 i ( 1 e τ = α ) i= 1 k a k b τ PART A RELAXING PLASTIC PAPERCLIP Consider an ordinary paperclip made of plastic, as they more
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF A LAMINATED BASALT COMPOSITE PLATE SUBJECTED TO BLAST LOAD
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 EXPERIMENTAL AND NUMERICAL ANALYSIS OF A LAMINATED BASALT COMPOSITE PLATE SUBJECTED TO BLAST LOAD Süleyman Baştürk 1,
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationTemperature Field Simulation of Polymeric Materials During Laser Machining Using COSMOS / M Software
Temperature Field Simulation of Polymeric Materials During Laser Machining Using COSMOS / M Software LIBUŠE SÝKOROVÁ, OLDŘICH ŠUBA, MARTINA MALACHOVÁ, JAKUB ČERNÝ Department of Production Engineering Tomas
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationSimulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias
As originally published in the IPC APEX EXPO Conference Proceedings. Simulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias Yan Ning, Michael H. Azarian, and Michael
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationFigure 1. Dimension of PSA in face paper laminate
EVALUATION OF DYNAMIC MECHANICAL PROPERTIES OF PRESSURE SENSITIVE ADHESIVE IN PAPER LANIMATES FOR POSTAGE STAMP APPLICATION: METHOD DEVELOPMENT AND ADHESIVE CHARACTERIZATION Hailing Yang, Graduate Student,
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationFinite Element Modeling of an Aluminum Tricycle Frame
Finite Element Modeling of an Aluminum Tricycle Frame A. Rodríguez, B. Chiné*, and J. A. Ramírez Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationAn Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire. Ziqing Yu¹ and Aixi Zhou²
An Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire Ziqing Yu¹ and Aixi Zhou² ¹Department of Engineering Technology, University of North Carolina at
More information